Download presentation

Presentation is loading. Please wait.

Published byMeghan Blair Modified over 2 years ago

1
First-principles study of the fcc/bcc interfaces Song Lu Material Science and Engineering, KTH-Royal institute of Technology, Sweden. Co-work with: Levente Vitos, Qing-miao Hu, Marko P. J. Punkkinen, Börje Johansson.

2
Coherent interface(Cu/Si) Semi-coherent interface(Fe/Cu, Cr/Ni, Cr/Cu, duplex steels, etc.) Incoherent interface (Cu-Nb) Introduction

3
An example in duplex stainless steel H. Jiao et al. Philo. Mag. 83, (2003)1867

4
Aims Calculate the lower and upper bounds of the interfacial energy. Calculate the lower and upper bounds of the work of separation.

5
Model system: Fe(110)/Ag(111) coherent interface Mismatch:~ 3.4% Mismatch: ~25%

6
Work of separation (W): the energy needed to separate the interface into two surfaces. (Here both the interface and the surfaces are constrained by the same lateral strain set by the underlying Ag lattice) The relationship between and W : Interfacial energy ( ): the energy needed to form the interface referred to the bulk states ’ Fe is the surface energy of Fe(110) calculated at strained state. (Ag underlylattice) ’ Ag is the surface energy of Ag(111) calculated at strained state. (Fe underlying lattice) OR

7
Taking Ag as underlying lattice:Taking Fe as underlying lattice: Fig. Map of the work of separation obtained by shifting the upper part against the lower part of the coherent interface when taking (a) Ag, (b) Fe as the underlying lattice, respectively. Result: Coherent work of separation

8
Underlying lattice W top W fcc W bridge W bcc top fcc bridge bcc Ag Fe Fe(110)1.642.182.022.241.320.790.940.720.512.45 Ag(111)1.432.212.04 1.130.360.53 0.681.88 Results for high-symmetric points Nonmagnetic: Fe 2.55 2.24

9
Averaging scheme for semicoherent/incoherent interface Work of separation (W) Interfacial energy ( ) Taking Ag as underlying lattice: Taking Fe as underlying lattice: For incoherent interface:

10
Semicoherent interface Underlying lattice: Ag Averaging scheme: W=1.91 Jm -2 = 0.65 Jm -2 Direct calculation: W=2.05 Jm -2 = 1.18 Jm -2 7% 70% Underlying lattice: Fe Averaging scheme: W=2.00 Jm -2 = 0.96 Jm -2 Direct calculation: W=2.08 Jm -2 = 1.10 Jm -2

11
Commensurate incoherent interface Putting the ideal (110)Fe on the ideal (111) Ag plane in the N-W orientation relationship without straining both lattices.

12
Ag underlying lattice:. Fe underlying lattice: J m -2.

13
Summary Using first-principles method, we can define the lower bound of the interfacial energy of the fcc/bcc interface, and the upper bound maybe properly estimated by an averaging scheme.

14
Thanks for your attention!

15
Strained surface energy ‘ Fe

16
Coherent Incoherent H. Jiao et al. Philo. Mag. 83, (2003)1867

17
Nonmagnetic: Fe 2.55 2.24

18
To describe an interface Habit plane: the plane of the plate of a plate-shaped crystal precipitate Orientation relationship: Kurdjumov–Sachs (K–S), Nishiyama– Wassermann (N-W) 5.26

Similar presentations

OK

Crystal-Air surface Interphase boundary Grain boundary Twin Boundary Stacking Faults Crystal Boundary Crystal-Crystal Low angle High angle 2D DEFECTS (Surface.

Crystal-Air surface Interphase boundary Grain boundary Twin Boundary Stacking Faults Crystal Boundary Crystal-Crystal Low angle High angle 2D DEFECTS (Surface.

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on rational numbers for class 9 Ppt on mass production Ppt on network switching techniques Ppt on no use of plastic bags Seminar ppt on smart card technology Ppt on low level language in computer Ppt on metro rail in hyderabad india Ppt on wireless network technologies Ppt on consistent and inconsistent equations Ppt on sources of energy for class 8th physics